Multifunctionality and Crystal Dynamics of a Highly Stable, Porous Metal-Organic Framework [Zn4O(NTB)2]
Eun Young Lee; Seung Yeon Jang; Myunghyun Paik Suh; Journal of the American Chemical Society 127 (2005) 6374–6381; doi:10.1021/ja043756x

data_4111647
_publ_contact_author_address
'School of Chemistry, Seoul National University'
_publ_contact_author_email       mpsuh@snu.ac.kr
_publ_contact_author_fax         '+82 2 886 8516'
_publ_contact_author_name        'Myunghyun Paik Suh (Prof.)'
_publ_contact_author_phone       '+82 2 880 7760'
_publ_section_title
;
 Multifunctionality and Crystal Dynamics of a Highly Stable, Porous
 Metal-Organic Framework [Zn4O(NTB)2]
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              6374
_journal_page_last               6381
_journal_paper_doi               10.1021/ja043756x
_journal_volume                  127
_journal_year                    2005
_chemical_formula_sum            'C42 H24 N2 O13 Zn4'
_chemical_formula_weight         1026.22
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           205
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P a -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 90.000(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            24
_cell_length_a                   22.393(5)
_cell_length_b                   22.393(5)
_cell_length_c                   22.393(5)
_cell_measurement_temperature    293(2)
_cell_volume                     11229(4)
_computing_molecular_graphics    'ORTEP-3 for Windows (Farrugia, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0486
_diffrn_reflns_av_sigmaI/netI    0.0675
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            6952
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_diffrn_reflns_theta_min         1.57
_exptl_absorpt_coefficient_mu    1.738
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    1.214
_exptl_crystal_description       rod-like
_exptl_crystal_F_000             4112
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.971
_refine_diff_density_min         -1.691
_refine_diff_density_rms         0.418
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.152
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     168
_refine_ls_number_reflns         4287
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.152
_refine_ls_R_factor_all          0.1584
_refine_ls_R_factor_gt           0.0720
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1152P)^2^+13.7444P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1888
_refine_ls_wR_factor_ref         0.2537
_reflns_number_gt                2367
_reflns_number_total             4287
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja043756xsi20041025_020245.cif
_cod_data_source_block           '[Zn4O(NTB)2]__(1')'
_cod_database_code               4111647